Download presentation

Presentation is loading. Please wait.

Published byZoey Millen Modified about 1 year ago

1
Chapter 3 -1 ISSUES TO ADDRESS... How do atoms assemble into solid structures? How does the density of a material depend on its structure? When do material properties vary with the sample (i.e., part) orientation? Chapter 3: The Structure of Crystalline Solids

2
Chapter 3 -2 Non dense, random packing Dense, ordered packing Dense, ordered packed structures tend to have lower energies. Energy and Packing Energy r typical neighbor bond length typical neighbor bond energy Energy r typical neighbor bond length typical neighbor bond energy

3
Chapter 3 -3 atoms pack in periodic, 3D arrays Crystalline materials... -metals -many ceramics -some polymers atoms have no periodic packing Noncrystalline materials... -complex structures -rapid cooling crystalline SiO 2 noncrystalline SiO 2 "Amorphous" = Noncrystalline Adapted from Fig. 3.23(b), Callister & Rethwisch 8e. Adapted from Fig. 3.23(a), Callister & Rethwisch 8e. Materials and Packing SiOxygen typical of: occurs for:

4
Chapter 3 -4 Metallic Crystal Structures How can we stack metal atoms to minimize empty space? 2-dimensions vs. Now stack these 2-D layers to make 3-D structures

5
Chapter 3 -5 Tend to be densely packed. Reasons for dense packing: - Typically, only one element is present, so all atomic radii are the same. - Metallic bonding is not directional. - Nearest neighbor distances tend to be small in order to lower bond energy. - Electron cloud shields cores from each other Have the simplest crystal structures. We will examine three such structures... Metallic Crystal Structures

6
Chapter 3 -6 Rare due to low packing density (only Po has this structure) Close-packed directions are cube edges. Coordination # = 6 (# nearest neighbors) Simple Cubic Structure (SC) Click once on image to start animation (Courtesy P.M. Anderson)

7
Chapter 3 -7 APF for a simple cubic structure = 0.52 APF = a 3 4 3 (0.5a) 3 1 atoms unit cell atom volume unit cell volume Atomic Packing Factor (APF) APF = Volume of atoms in unit cell* Volume of unit cell *assume hard spheres Adapted from Fig. 3.24, Callister & Rethwisch 8e. close-packed directions a R=0.5a contains 8 x 1/8 = 1atom/unit cell

8
Chapter 3 -8 Coordination # = 8 Adapted from Fig. 3.2, Callister & Rethwisch 8e. Atoms touch each other along cube diagonals. --Note: All atoms are identical; the center atom is shaded differently only for ease of viewing. Body Centered Cubic Structure (BCC) ex: Cr, W, Fe ( ), Tantalum, Molybdenum 2 atoms/unit cell: 1 center + 8 corners x 1/8 Click once on image to start animation (Courtesy P.M. Anderson)

9
Chapter 3 -9 Atomic Packing Factor: BCC a APF = 4 3 (3a/4) 3 2 atoms unit cell atom volume a 3 unit cell volume length = 4R = Close-packed directions: 3 a APF for a body-centered cubic structure = 0.68 a R Adapted from Fig. 3.2(a), Callister & Rethwisch 8e. a 2 a 3

10
Chapter 3 -10 Coordination # = 12 Adapted from Fig. 3.1, Callister & Rethwisch 8e. Atoms touch each other along face diagonals. --Note: All atoms are identical; the face-centered atoms are shaded differently only for ease of viewing. Face Centered Cubic Structure (FCC) ex: Al, Cu, Au, Pb, Ni, Pt, Ag 4 atoms/unit cell: 6 face x 1/2 + 8 corners x 1/8 Click once on image to start animation (Courtesy P.M. Anderson)

11
Chapter 3 -11 APF for a face-centered cubic structure = 0.74 Atomic Packing Factor: FCC maximum achievable APF APF = 4 3 (2a/4) 3 4 atoms unit cell atom volume a 3 unit cell volume Close-packed directions: length = 4R = 2 a Unit cell contains: 6 x 1/2 + 8 x 1/8 =4 atoms/unit cell a 2 a Adapted from Fig. 3.1(a), Callister & Rethwisch 8e.

12
Chapter 3 -12 A sites B B B B B BB C sites C C C A B B ABCABC... Stacking Sequence 2D Projection FCC Unit Cell FCC Stacking Sequence B B B B B BB B sites C C C A C C C A

13
Chapter 3 -13 Coordination # = 12 ABAB... Stacking Sequence APF = 0.74 3D Projection 2D Projection Adapted from Fig. 3.3(a), Callister & Rethwisch 8e. Hexagonal Close-Packed Structure (HCP) 6 atoms/unit cell ex: Cd, Mg, Ti, Zn c/a = 1.633 c a A sites B sites A sites Bottom layer Middle layer Top layer

14
Chapter 3 -14 Theoretical Density, where n = number of atoms/unit cell A = atomic weight V C = Volume of unit cell = a 3 for cubic N A = Avogadro’s number = 6.022 x 10 23 atoms/mol Density = = VC NAVC NA n An A = Cell Unit of VolumeTotal Cell Unit in Atomsof Mass

15
Chapter 3 -15 Ex: Cr (BCC) A = 52.00 g/mol R = 0.125 nm n = 2 atoms/unit cell theoretical a = 4R/ 3 = 0.2887 nm actual a R = a3a3 52.002 atoms unit cell mol g unit cell volume atoms mol 6.022 x 10 23 Theoretical Density, = 7.18 g/cm 3 = 7.19 g/cm 3 Adapted from Fig. 3.2(a), Callister & Rethwisch 8e.

16
Chapter 3 -16 Densities of Material Classes metals > ceramics > polymers Why? Data from Table B.1, Callister & Rethwisch, 8e. (g/cm ) 3 Graphite/ Ceramics/ Semicond Metals/ Alloys Composites/ fibers Polymers 1 2 20 30 Based on data in Table B1, Callister *GFRE, CFRE, & AFRE are Glass, Carbon, & Aramid Fiber-Reinforced Epoxy composites (values based on 60% volume fraction of aligned fibers in an epoxy matrix). 10 3 4 5 0.3 0.4 0.5 Magnesium Aluminum Steels Titanium Cu,Ni Tin, Zinc Silver, Mo Tantalum Gold, W Platinum Graphite Silicon Glass-soda Concrete Si nitride Diamond Al oxide Zirconia HDPE, PS PP, LDPE PC PTFE PET PVC Silicone Wood AFRE* CFRE* GFRE* Glass fibers Carbonfibers Aramid fibers Metals have... close-packing (metallic bonding) often large atomic masses Ceramics have... less dense packing often lighter elements Polymers have... low packing density (often amorphous) lighter elements (C,H,O) Composites have... intermediate values In general

17
Chapter 3 -17 Some engineering applications require single crystals: Properties of crystalline materials often related to crystal structure. (Courtesy P.M. Anderson) -- Ex: Quartz fractures more easily along some crystal planes than others. -- diamond single crystals for abrasives -- turbine blades Fig. 8.33(c), Callister & Rethwisch 8e. (Fig. 8.33(c) courtesy of Pratt and Whitney). (Courtesy Martin Deakins, GE Superabrasives, Worthington, OH. Used with permission.) Crystals as Building Blocks

18
Chapter 3 -18 Most engineering materials are polycrystals. Nb-Hf-W plate with an electron beam weld. Each "grain" is a single crystal. If grains are randomly oriented, overall component properties are not directional. Grain sizes typically range from 1 nm to 2 cm (i.e., from a few to millions of atomic layers). Adapted from Fig. K, color inset pages of Callister 5e. (Fig. K is courtesy of Paul E. Danielson, Teledyne Wah Chang Albany) 1 mm Polycrystals Isotropic Anisotropic

19
Chapter 3 -19 Single Crystals -Properties vary with direction: anisotropic. -Example: the modulus of elasticity (E) in BCC iron: Data from Table 3.3, Callister & Rethwisch 8e. (Source of data is R.W. Hertzberg, Deformation and Fracture Mechanics of Engineering Materials, 3rd ed., John Wiley and Sons, 1989.) Polycrystals -Properties may/may not vary with direction. -If grains are randomly oriented: isotropic. (E poly iron = 210 GPa) -If grains are textured, anisotropic. 200 m Adapted from Fig. 4.14(b), Callister & Rethwisch 8e. (Fig. 4.14(b) is courtesy of L.C. Smith and C. Brady, the National Bureau of Standards, Washington, DC [now the National Institute of Standards and Technology, Gaithersburg, MD].) Single vs Polycrystals E (diagonal) = 273 GPa E (edge) = 125 GPa

20
Chapter 3 -20 Polymorphism Two or more distinct crystal structures for the same material (allotropy/polymorphism) titanium , -Ti carbon diamond, graphite BCC FCC BCC 1538ºC 1394ºC 912ºC - Fe - Fe - Fe liquid iron system

21
Chapter 3 -21 Fig. 3.4, Callister & Rethwisch 8e. Crystal Systems 7 crystal systems 14 crystal lattices Unit cell: smallest repetitive volume which contains the complete lattice pattern of a crystal. a, b, and c are the lattice constants

22
Chapter 3 -22 Point Coordinates Point coordinates for unit cell center are a/2, b/2, c/2 ½ ½ ½ Point coordinates for unit cell corner are 111 Translation: integer multiple of lattice constants identical position in another unit cell z x y a b c 000 111 y z 2c2c b b

23
Chapter 3 -23 Crystallographic Directions -4, 1, 2 families of directions z x where the overbar represents a negative index [ 412 ] => y Example 2: pt. 1 x 1 = a, y 1 = b /2, z 1 = 0 pt. 2 x 2 = - a, y 2 = b, z 2 = c => -2, 1/2, 1 pt. 2 head pt. 1: tail Multiplying by 2 to eliminate the fraction

24
Chapter 3 -24 Crystallographic Directions 1. Vector repositioned (if necessary) to pass through origin. 2. Read off projections in terms of unit cell dimensions a, b, and c 3. Adjust to smallest integer values 4. Enclose in square brackets, no commas [uvw] ex: 1, 0, ½=> 2, 0, 1=> [ 201 ] -1, 1, 1 families of directions z x Algorithm where overbar represents a negative index [ 111 ] => y

25
Chapter 3 -25 ex: linear density of Al in [110] direction a = 0.405 nm Linear Density Linear Density of Atoms LD = a [110] Unit length of direction vector Number of atoms # atoms length 1 3.5 nm a2 2 LD Adapted from Fig. 3.1(a), Callister & Rethwisch 8e.

26
Chapter 3 -26 HCP Crystallographic Directions 1. Vector repositioned (if necessary) to pass through origin. 2. Read off projections in terms of unit cell dimensions a 1, a 2, a 3, or c 3. Adjust to smallest integer values 4. Enclose in square brackets, no commas [uvtw] [ 1120 ]ex: ½, ½, -1, 0 => Adapted from Fig. 3.8(a), Callister & Rethwisch 8e. dashed red lines indicate projections onto a 1 and a 2 axes a1a1 a2a2 a3a3 -a3-a3 2 a 2 2 a 1 - a3a3 a1a1 a2a2 z Algorithm

27
Chapter 3 -27 HCP Crystallographic Directions Hexagonal Crystals –4 parameter Miller-Bravais lattice coordinates are related to the direction indices (i.e., u'v'w') as follows. 'ww t v u )vu( +- )'u'v2( 3 1 - )'v'u2( 3 1 - ]uvtw[]'w'v'u[ Fig. 3.8(a), Callister & Rethwisch 8e. - a3a3 a1a1 a2a2 z

28
Chapter 3 -28 Crystallographic Planes Adapted from Fig. 3.10, Callister & Rethwisch 8e.

29
Chapter 3 -29 Crystallographic Planes Miller Indices: Reciprocals of the (three) axial intercepts for a plane, cleared of fractions & common multiples. All parallel planes have same Miller indices. Algorithm 1. Read off intercepts of plane with axes in terms of a, b, c 2. Take reciprocals of intercepts 3. Reduce to smallest integer values 4. Enclose in parentheses, no commas i.e., (hkl)

30
Chapter 3 -30 Crystallographic Planes z x y a b c 4. Miller Indices (110) examplea b c z x y a b c 4. Miller Indices (100) 1. Intercepts 1 1 2. Reciprocals 1/1 1/1 1/ 1 1 0 3. Reduction 1 1 0 1. Intercepts 1/2 2. Reciprocals 1/½ 1/ 1/ 2 0 0 3. Reduction 2 0 0 examplea b c

31
Chapter 3 -31 Crystallographic Planes z x y a b c 4. Miller Indices (634) example 1. Intercepts 1/2 1 3/4 a b c 2. Reciprocals 1/½ 1/1 1/¾ 21 4/3 3. Reduction 63 4 (001)(010), Family of Planes {hkl} (100),(010),(001),Ex: {100} = (100),

32
Chapter 3 -32 Crystallographic Planes (HCP) In hexagonal unit cells the same idea is used example a 1 a 2 a 3 c 4. Miller-Bravais Indices(1011) 1. Intercepts 1 1 2. Reciprocals 1 1/ 1 0 1 1 3. Reduction1 0 1 a2a2 a3a3 a1a1 z Adapted from Fig. 3.8(b), Callister & Rethwisch 8e.

33
Chapter 3 -33 Crystallographic Planes We want to examine the atomic packing of crystallographic planes Iron foil can be used as a catalyst. The atomic packing of the exposed planes is important. a)Draw (100) and (111) crystallographic planes for Fe. b) Calculate the planar density for each of these planes.

34
Chapter 3 - Virtual Materials Science & Engineering (VMSE) 34 VMSE is a tool to visualize materials science topics such as crystallography and polymer structures in three dimensions Available in Student Companion Site at www.wiley.com/college/callister and in WileyPLUS

35
Chapter 3 - VMSE: Metallic Crystal Structures & Crystallography Module 35 VMSE allows you to view crystal structures, directions, planes, etc. and manipulate them in three dimensions

36
Chapter 3 - Unit Cells for Metals 36 VMSE allows you to view the unit cells and manipulate them in three dimensions Below are examples of actual VMSE screen shots FCC StructureHCP Structure

37
Chapter 3 - VMSE: Crystallographic Planes Exercises 37 Additional practice on indexing crystallographic planes

38
Chapter 3 -38 Planar Density of (100) Iron Solution: At T < 912ºC iron has the BCC structure. (100) Radius of iron R = 0.1241 nm R 3 34 a Adapted from Fig. 3.2(c), Callister & Rethwisch 8e. 2D repeat unit = Planar Density = a 2 1 atoms 2D repeat unit = nm 2 atoms 12.1 m2m2 atoms = 1.2 x 10 19 1 2 R 3 34 area 2D repeat unit

39
Chapter 3 -39 Planar Density of (111) Iron Solution (cont): (111) plane 1 atom in plane/ unit surface cell 33 3 2 2 R 3 16 R 3 4 2 a3ah2area atoms in plane atoms above plane atoms below plane ah 2 3 a 2 2D repeat unit 1 = = nm 2 atoms 7.0 m2m2 atoms 0.70 x 10 19 3 2 R 3 16 Planar Density = atoms 2D repeat unit area 2D repeat unit

40
Chapter 3 - VMSE Planar Atomic Arrangements 40 VMSE allows you to view planar arrangements and rotate them in 3 dimensions BCC (110) Plane

41
Chapter 3 -41 X-Ray Diffraction Diffraction gratings must have spacings comparable to the wavelength of diffracted radiation. Can’t resolve spacings Spacing is the distance between parallel planes of atoms.

42
Chapter 3 -42 X-Rays to Determine Crystal Structure X-ray intensity (from detector) c d d n 2 sin c Measurement of critical angle, c, allows computation of planar spacing, d. Incoming X-rays diffract from crystal planes. Adapted from Fig. 3.20, Callister & Rethwisch 8e. reflections must be in phase for a detectable signal spacing between planes d incoming X-rays outgoing X-rays detector extra distance travelled by wave “2” “1” “2” “1” “2”

43
Chapter 3 -43 X-Ray Diffraction Pattern Adapted from Fig. 3.22, Callister 8e. (110) (200) (211) z x y a b c Diffraction angle 2 Diffraction pattern for polycrystalline -iron (BCC) Intensity (relative) z x y a b c z x y a b c

44
Chapter 3 -44 SUMMARY Atoms may assemble into crystalline or amorphous structures. We can predict the density of a material, provided we know the atomic weight, atomic radius, and crystal geometry (e.g., FCC, BCC, HCP). Common metallic crystal structures are FCC, BCC, and HCP. Coordination number and atomic packing factor are the same for both FCC and HCP crystal structures. Crystallographic points, directions and planes are specified in terms of indexing schemes. Crystallographic directions and planes are related to atomic linear densities and planar densities.

45
Chapter 3 -45 Some materials can have more than one crystal structure. This is referred to as polymorphism (or allotropy). SUMMARY Materials can be single crystals or polycrystalline. Material properties generally vary with single crystal orientation (i.e., they are anisotropic), but are generally non-directional (i.e., they are isotropic) in polycrystals with randomly oriented grains. X-ray diffraction is used for crystal structure and interplanar spacing determinations.

46
Chapter 3 -46 Core Problems: Self-help Problems: ANNOUNCEMENTS Reading:

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google